Integration of Environmental Friendly Perovskites for High-efficiency White Light-emitting Diodes
Nanoscale Research Letters
December 2019, 14:152 | Cite as
Integration of Environmental Friendly Perovskites for High-efficiency White Light-emitting Diodes
AuthorsAuthors and affiliations
Hanxin LiuChun SunZhiyuan GaoChong GengShuangshuang ShiLe WangSijing SuWengang Bi
First Online: 02 May 2019
Perovskite quantum dots (QDs) have been widely used in white light-emitting diodes (WLEDs), due to their high quantum yield (QY), tunable bandgap, and simple preparation. However, the red-emitting perovskite QDs are usually containing iodine (I), which is not stable under continuous light irradiation. Herein, perovskite-based WLED is fabricated by lead-free bismuth (Bi)-doped inorganic perovskites Cs2SnCl6 and less-lead Mn-doped CsPbCl3 QDs, which emits white light with color coordinates of (0.334, 0.297). The Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3 QDs both show excellent stability when kept in the ambient air. As benefits from this desired characteristic, the as-prepared WLED shows excellent stability along with operating time. These results can promote the application of inorganic perovskite QDs in the field of WLEDs.
KeywordsQuantum dots perovskite WLED doping
White light-emitting diodes
Power conversion efficiency
Lead (II) chloride
Manganese chloride tetrahydrate
Time-resolved PL spectroscopy
Transmission electron microscope
Scanning electron microscope
Energy dispersive X-ray detector
Full width at half maximum
High-resolution transmission electron microscopy
Selected area electron diffraction
Among solid-state lighting technology, white light-emitting diodes (WLEDs) are excellent candidates to replace incandescent lamps for their merits of high-energy conservation, long lifetime, high luminous efficiency, and polarized emissions . In general, WLEDs were recognized as one kind of the economical and efficient solid-state lighting sources [2, 3]. QD-LED technology is gradually developed over the past few years, because of high stability and high quantum yield (QY) of quantum dots (QDs) . Recently, perovskites have attracted much attention, and they have been applied in many different fields [5, 6, 7, 8, 9, 10, 11, 12, 13, 14, 15]. Perovskite solar cells with power conversion efficiency (PCE) exceeding 23% have been achieved because of their excellent absorption (Abs) coefficients, long carrier diffusion lengths, and high carrier mobilities [5, 6, 7]. CsPbBr3-encapsulated PbSe wires have shown good optoelectronic performance including high responsivity (~ 104 A W−1) and fair response speed (~ ms), demonstrating their great potential application in photodetection fields [8, 9, 10]. Additionally, perovskites have been introduced into photonic devices. The remarkable features of perovskite, such as rich phase compositions and low-temperature solution process ability, made perovskite can be applied in transistors . Low-threshold amplified spontaneous emission and lasing can be realized by CsPbX3 QDs . Most of all, perovskite QDs are the most promising material among QDs for LED application, due to high QY (up to > 90%), intense photoluminescence (PL), simple preparation procedure, and highly tunable bandgaps (from 1.46 to 2.50 ev) [11, 12, 13, 14, 15, 16]. However, the anion-exchange reaction between perovskites and instability of iodine (I)-containing perovskite largely restricted the development of perovskite QDs toward WLED application. Sun et al. proposed to use silica encapsulation to enhance stability and avoid anion exchange . The air stability of perovskite QDs was enhanced greatly, but the WLED stability is not good enough because of the significant dropping of red light. Then, Shen et al. used the anthracene shell to protect red-emitting perovskite QDs, which enhanced the LED stability against current . Zhong and coworkers directly used red-emitting K2SiF6:Mn4+ phosphor to replace iodine (I)-containing perovskite QDs . Sun and coworkers also presented the same method to enhance the stability of LED . Due to the sharp emission lines of perovskite QDs, they usually are used in backlight display application with blue-emitting LED chips [21, 22]. These WLEDs are not proper for solid-state lighting, because their CRI is quite low. Recently, several reports have prepared single-phase phosphor of perovskites, which possess broad linewidths. However, the QYs of this kind of material are relatively low [23, 24, 25]. Another great problem is that the perovskite QDs contain lead, which is poison to health and environment [26, 27]. With the growing concerns about this risk, restrictions have been made to limit the use of Pb in consumer electronics. A lot of efforts have been done to explore and replace lead with less toxic elements like Sn, Ge, Bi, and Sb, which have analogous electronic band structure [28, 29, 30]. However, their optoelectronic properties cannot be comparable with the Pb-based counterparts. Doping less toxic elements into perovskite lattice has been an alternative route, which can introduce new optical, electronic, and magnetic properties [31, 32]. For example, Zhang et al. have prepared Mn-doped perovskite QDs with QYs up to 54% and the highest Mn substitution ratio was 46% . Tang and coworkers reported Bi-doped lead-free inorganic perovskites. After doping Bi, the PLQY of Bi-doped Cs2SnCl6 is enhanced to 78.9% .
In this work, we introduce Mn-doped CsPbCl3 QDs and Bi-doped Cs2SnCl6 as the orange emission light and blue emission light to fabricate high-performance WLEDs. These two materials both can be excited by UV light and exhibit high QYs under UV light. They also contain the same anion Cl, which avoids the anion exchange reaction during the mixing process. Besides, it is worth to note that the emission linewidths of these two perovskites are very broad, which facilitate to form a continuous spectrum. In a WLED with a CCT of 5311K, the color coordinates of (0.334, 0.297) and CRI of 80 were achieved. Most of all, this WLED showed excellent stability against increasing currents and working time.
Materials and Chemicals
Cesium carbonate (Cs2CO3, 99.9%), lead (II) chloride (PbCl2, 99.999%), cesium chloride (CsCl, 99.99%), oleic acid (OA, 90%), and 1-octadecene (ODE, 90%) were obtained from Alfa Aesar. Manganese chloride tetrahydrate (MnCl2·(H2O)4, 99.99%), oleylamine (OAm, 80–90%), and tin chloride (SnCl2, 99.99%) were purchased from Aladdin. Bismuth chloride (BiCl3, 99.99%) and polymethyl methacrylate (PMMA) were obtained from Macklin. Hydrochloric acid (HCl, 37 wt.% in water) was purchased from Sinopharm Chemical Reagent Co., Ltd. Methanol (99.5%) was obtained from Kermel. Toluene (99.0%) and ethyl acetate (99.5%) were purchased from Concord. Hexane was obtained from Beijing Chemical Factory.
Preparation of Cs-oleate
The cesium-oleate solution was prepared according to the approach by Kovalenko and co-workers . In brief, 0.8 g of Cs2CO3, 2.5 mL of OA, and 30 mL of ODE were loaded in a three-neck flask and dried under vacuum at 120 °C for 1 h. Next, the flask was switched to N2 atmosphere and heated to 150 °C until all the Cs2CO3 dissolved.
Synthesis of Mn-doped CsPbCl3
The Mn-doped CsPbCl3 was synthesized by hot injection method. Typically, 0.0615 g of PbCl2, 0.08 g of MnCl2 (H2O)4, 1 ml of OAm, 1 ml of OA, and 5 ml of ODE were added to a 25-mL three-neck flask and dried in a vacuum at 120 °C for 1 h. And then, the flask was heated up to 180 °C under nitrogen. At this temperature, 0.5 mL of dried OAm and 0.5 mL of dried OA were subsequently injected to solubilize the Pb and Mn sources. Then, 0.4 mL of Cs-oleate was swiftly injected, and after 5 s, the solution was cooled with an ice bath. The QDs were precipitated with hexanes and ethyl acetate by the ratio of 1:3. Then, the solution was centrifuged at 5500 rpm for 5 min. After centrifugation, the precipitates were dispersed in toluene.
Synthesis of Bi-doped Cs2SnCl6
The Bi-doped Cs2SnCl6 was synthesized by hydrothermal reaction method. Typically, 0.337 g of CsCl, 0.189 g of SnCl2, 0.032 g of BiCl3 powders, and 4.0 mL of 37% hydrochloric acid were sealed into a Teflon-lined autoclave (30 mL) and heated at 220 °C for 20 h. After the reaction, the autoclave was slowly cooled to room temperature, and a white crystal of Bi-doped Cs2SnCl6 could be separated by centrifugation (3000 rpm, 2 min).
Fabrication of LED Devices
UV-LED chips with an emission peak wavelength centered at 365 nm were purchased from Shine On Corp. In a typical preparation, a certain amount of Bi-doped Cs2SnCl6 powder was mixed with PMMA/toluene solution and coated onto the UV-LED chip. Next, Mn-Doped CsPbCl3 QD solution was added into a 1-ml transparent PMMA/toluene solution. After that, the Mn-doped CsPbCl3 solution was coated onto the UV-LED chip which was already coated with Bi-doped Cs2SnCl6. The device was then cured at room temperature for 30 min.
Measurement and Characterization
Fluorescence emission spectra were conducted on an Ocean Optics spectrometer. Absorbance spectra of samples were measured by using a Shimadzu UV-2550 spectrophotometer. For Bi-doped Cs2SnCl6 diffuse reflectance (R) spectra were measured by Ocean Optics spectrometer, and the Abs coefficient α was obtained by using the Kubelka–Munk theory (1 − R) × (1 − R)/2R. The excitation spectra and time-resolved PL spectroscopy (TRPL) have been measured by an Edinburgh FLS920 fluorescence spectrometer. The morphology of the QDs was acquired by a FEI Tecnai G2 Spirit TWIN transmission electron microscope (TEM) operating at 100 kV. Scanning electron microscope (SEM) and energy-dispersive X-ray spectroscopy (EDX) measurement have been performed by Quanta 450 FEG. X-ray diffraction (XRD) patterns of perovskites were carried out using a Bruker D8 Advance X-ray diffractometer (Cu Kα: λ = 1.5406 Å). The absolute PL QYs of the samples were obtained by a fluorescence spectrometer (FLS920P, Edinburgh Instruments) equipped with an integrating sphere with its inner face coated with BENFLEC. The brightness and efficiency have been measured by ATA-1000 electroluminescence measurement system (Everfine in People’s Republic of China).
Results and Discussion
Bi-doped Cs2SnCl6 perovskite was synthesized according to the previous approach with little modification . The Abs and PL spectra of Bi-doped Cs2SnCl6 are presented in Fig. 1a. As shown in Fig. 1a, the sharp Abs peak at around 375 nm could be assigned to the transitions from the defect band (caused by Bi doping) to the host conduction band minimum, which is in good accordance with previous reports . The XRD pattern also indicates the formation of Sn-based perovskite (Fig. 3a). All the diffraction peaks matched well with the Cs2SnCl6 crystal structure (ICSD #9023), and no impurity phases were detected, which is in good accordance with a previous report . The Bi-doped Cs2SnCl6 can be excited by UV light (365 nm) and exhibits bright blue light with the PL emission peak located at 465 nm (Fig. 1a). The full width at half maximum (FWHM) of Bi-doped Cs2SnCl6 is 65 nm, and the QY of Bi-doped Cs2SnCl6 is up to 76%. The PL excitation (PLE) spectrum of Bi-doped Cs2SnCl6 has been measured (detected at 465 nm) and shown in Fig. 1a. A broad peak located at 350 nm can be observed in the PLE spectrum of Bi-doped Cs2SnCl6, which shifts slightly compared to the Abs spectrum. The similar variation was observed by a previous report . In addition, this Bi-doped Cs2SnCl6 shows excellent stability. After being irradiated for 300 h with UV light, the PL intensity is nearly constant. The perovskite powder can maintain its QY after being exposed to air for 3 months (25 °C, relative humidity 35–50%).
Open image in new window
a Abs, PL, and PLE spectra of Bi-doped Cs2SnCl6 QDs. The inset is the photograph of the sample under UV excitation. b Abs, PL, and PLE spectra of Mn-doped CsPbCl3 QDs. The inset is the photograph of the sample under UV excitation
Mn-doped CsPbCl3 QDs were prepared according to an established process with minor modification . As shown in Fig. 1b, the Abs peak at around 400 nm is observed, which is assigned to exciton Abs of CsPbCl3. Under UV light (365 nm), the QD solution shows a bright orange emission (Fig. 1b, inset). Two peaks are observed in the PL emission spectrum, which center at 405 nm and 595 nm, respectively (Fig. 1b). The peak at 405 nm is assigned to the CsPbCl3 host, while the broad emission band with the FWHM at about 80 nm is assigned to Mn2+ d-d emission [31, 34]. The QY of our product is reaching to 52%, which is comparable with other reports [32, 35, 36]. The PLE spectrum of Mn-doped CsPbCl3 has been measured (detected at 595 nm) and shown in Fig. 1b. The PLE spectrum of Mn-doped CsPbCl3 closely follows the Abs spectrum, which demonstrates that the strong PL peak of the Mn emission originates from the exciton of perovskite. The as-prepared QDs show excellent stability, which can preserve their emission properties under ambient atmospheres for at least 3 months (25 °C, relative humidity 35–50%).
The PL lifetimes of Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3 were measured using TRPL. As shown in Fig. 2a, the decay curve of Bi-doped Cs2SnCl6 is fitted well by an exponential function and the lifetime is 375 ns, which is in good accordance with the previous report . As for Mn-doped CsPbCl3 QDs, the lifetime is longer (1.7 ms), which supports that it originates from the spin-forbidden ligand field transition of the Mn2+ ions .
Open image in new window
a PL decay and fitted curves of Bi-doped Cs2SnCl6. b PL decay and fitted curves of Mn-doped CsPbCl3
Figure 3b shows the SEM image of Bi-doped Cs2SnCl6 perovskite. The spherical Bi-doped Cs2SnCl6 perovskite with a diameter of 53 nm can be observed. EDX and mapping images further confirm the presence of Bi in Cs2SnCl6 (Fig. 3j, c–f). The ratio of Cs, Sn, Bi, and Cl is 1:0.62:0.14:3, which is in good accordance with other reports . Figure 3g shows the TEM image of Mn-doped CsPbCl3 QDs. As can be seen, the Mn-doped CsPbCl3 QDs show a cubic morphology with an average size of ∼ 12 nm. As can be seen from Fig. 3k, the ratio of Cs, Pb, Mn, and Cl is 1:0.77:0.19:2.68. The HRTEM image displays the lattice fringes of the Mn-doped CsPbCl3 QDs, which shows an interplanar distance of 3.67 Å, and matches well with that of the (101) plane (Fig. 3h). The SAED pattern is shown in Fig. 4c. We can see that the QDs possess a tetragonal crystal structure with corresponding (101) and (200) planes (Fig. 3i) . XRD pattern of the Mn-doped CsPbCl3 QDs shows that the diffraction peaks are corresponding to the tetragonal phase, which is consistent with the SAED results.
Open image in new window
a XRD patterns of Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3 QDs, b the SEM image of Bi-doped Cs2SnCl6, c–f the mapping images of Bi-doped Cs2SnCl6, g TEM image of Mn-doped CsPbCl3 perovskite QDs, h high-resolution transmission electron microscopy (HRTEM) image of Mn-doped CsPbCl3 QDs, i elected area electron diffraction (SAED) pattern of Mn-doped CsPbCl3, j the EDX spectrum and Bi-doped Cs2SnCl6, and k the EDX spectrum of Mn-doped CsPbCl3
Open image in new window
a PL spectra of Mn-doped CsPbCl3 QDs at different concentration. b Color coordinates variation of Mn-doped CsPbCl3 QDs at different concentration
In order to acquire the optimal Mn doping concentration, the emission peak and FWHM variation are analyzed and shown in Fig. 4. It can be seen from Fig. 4a that the PL intensity increases as the concentration of Mn2+ is increased from 3.04 to 6.45 mg/mL. Further increasing the Mn2+ concentration makes the PL intensity decrease, which is due to the self-Abs effect at high concentration. During the whole process, the PL peak position and the FWHM remains the same. In other words, the change of Mn2+ concentration has no effect on the PL emission peak and FWHM, which are also verified by the color coordinates chart (Fig. 4b). No matter how the concentration changes, the color coordinates are basically maintained at (0.535, 0.460) (the black dots). Therefore, the concentration of 6.45 mg/mL is taken as the optimal concentration.
A WLED was fabricated by coating blue-emitting Bi-doped Cs2SnCl6 powder and orange-emitting Mn-doped CsPbCl3 QDs onto a commercially available 365 nm LED chip (Fig. 5a). As shown in Fig. 5b, two obvious peaks can be seen from the EL spectrum of the WLED, which attribute to Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3. The perseverance of these two peaks indicates that no anion exchange and other chemical reactions occur in the fabrication process. In bright white light with color coordinates of (0.334, 0.297), the correlated color temperature of 5311 K can be observed when the WLED is operated at 15 mA (Fig. 5b and c). The highest luminous efficiency and luminance of the WLED reach up to 20.8 lm/W and 78,000 cd m−2, respectively, which are comparable with other UV chip-based WLEDs [4, 37, 38, 39].
Open image in new window
a Schematic of the fabrication process of the WLED; b electroluminescent (EL) spectrum of WLED; c color coordinates of WLED device, Mn-doped CsPbCl3 QDs, and Bi-doped Cs2SnCl6。 (the black dot inside the circle is the white color coordinates and the asterisk represents the blue and orange perovskite). The inserts are the photograph of the WLED
The emission spectra of the as-fabricated WLED with the driving currents of 5 mA-120 mA are given in Fig. 6a. The detailed characteristics including color coordinates, CCT, and CRI of the as-fabricated WLED are shown in Table 1. As shown in Fig. 6a, the EL intensities of both peaks increase gradually along with increasing the current and show no saturation. Besides, no obvious shift of the peak position for the EL spectrum occurred under different injection currents. Color coordinates of these PL spectra are shown in Fig. 6b. The chromaticity coordinates show little shift (x < 0.02, y < 0.02) to the left with increasing the driving currents. We can observe that the EL intensity of Bi-doped Cs2SnCl6 increases faster than that of the Mn-doped CsPbCl3, which can result in chromaticity coordinates moving left. However, the FWHM variation and the shift of emission peak also cause chromaticity coordinates to move. As we discussed above, the emission peak is unchanged with the increase of currents. Because of their broad FWHM, the emission peaks of Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3 overlap, which is difficult to analyze the FWHM variation. Therefore, monochromatic LEDs have been fabricated to analyze each FWHM variation. Figure 6c and d show the emission spectra of Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3 LEDs, respectively. In the wide current range from 5 to 120 mA, no shift of the PL emission peaks occurs, which is in good accordance with the WLED results (Fig. 6c and d). The FWHM variation of the coated LEDs under different currents is shown in Fig. 6e. As can be seen, the FWHMs of Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3 are nearly constant, indicating that the variation of chromaticity coordinates of the WLED only results from the change of intensity of the EL. The difference of EL intensity variation perhaps comes from the different thermal stability of Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3, because the increase of currents could result in the temperature of LED chip increasing. This insignificant change can be further alleviated by adopting a remote-type LED structure. Moreover, the long-term operating stability can be observed from Fig. 6f. After a continuous work of 300 h, the EL intensities of both Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3 are declined less than 10%. Actually, the half-life of the WLED is 3000 h, which is far better than I-containing perovskites [15, 17, 18, 40]. As can be seen from Table 2, after the as-prepared WLED continues working at 15 mA over 50 h, the PL intensity drops to 99% of the original, which is much better than other reports [17, 18, 36, 40, 41, 42, 43, 44]. After working 100 hours, the PL intensity only drops to 97%.
Open image in new window
a PL spectra of WLED device under different injection currents, b chromaticity coordinates change of WLED device under different injection currents, c PL spectra of Bi-doped Cs2SnCl6 LED device under different injection currents, d PL spectra of Mn-doped CsPbCl3 LED device under different injection currents, e the FWHM variation of Bi-doped Cs2SnCl6 and Mn-doped CsPbCl3, f the PL intensity variation measured at different working time intervals
Color coordinates (x, y), CCT, and Ra of the WLED device under different injection currents
Comparison of different WLEDs fabricated by perovskite
PL intensity, working time
10 h, 83%
2.7% Ce/9.1% Mn co-doped CsPbCl1.8Br1.2
20 h, 89%
Mn2+-doped CsPb (Cl0.5Br0.5)3
24 h, 96%
100 h, 73%
30 h, 83.5%
30 min, 80%
13 h, 96%
50 h, 97%
50 h, 99%
100 h, 97%
Nowadays, perovskite heterojunctions have been adopted to improve the physical properties of perovskite [45, 46]. Usually, these heterojunctions can integrate the merits of both materials, such as perovskite-polymer bulk heterostructure, perovskite-PbS core-shell structure, and perovskite-plasmonic Au or Ag composite material [47, 48, 49], which can enhance efficiency. However, due to the poor stability of perovskite, it is difficult to design and fabricate heterojunction. Besides, these perovskite heterojunctions may be not stable compared to pure perovskite.
In conclusion, we have combined high-quality blue-emitting bismuth-doped Cs2SnCl6 perovskite with orange-emitting Mn-doped CsPbCl3 QDs to fabricate WLED. Because they all contain the same anion of Cl, anion exchange reaction can be avoided. Besides, orange-emitting Mn-doped CsPbCl3 QDs show better stability compared with iodine-containing counterparts. The WLED with color coordinates of (0.334, 0.297) is acquired by tuning the ratio of them. In addition, the WLED show excellent long-term operating stability, which is by far, to our knowledge, the most stable one among perovskite-based WLEDs. We believe our findings will open up new avenues for the exploration of novel lead-free perovskite-based WLED.
This study was supported by the Natural Science Foundation of Hebei Province (F2018202046) and State Key Laboratory of Reliability and Intelligence of Electrical Equipment (EERIZZ2018003).
This study was funded by the Natural Science Foundation of Hebei Province (F2018202046) and State Key Laboratory of Reliability and Intelligence of Electrical Equipment (EERIZZ2018003).
Availability of Data and Materials
The datasets generated during and/or analyzed during the current study are available from the corresponding authors on reasonable request.
HL, CS, and WB conceived and designed the experiments. HL performed the experiments and analyzed the data. ZG, CG, SS, LW, and SS contributed to the analysis tools. HL and CS wrote the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Schubert EF, Kim JK (2005) Solid-state light sources getting smart. Science 308:1274–1278CrossRefGoogle Scholar
Chen LY, Chang JK, Cheng WC et al (2015) Chromaticity tailorable glass-based phosphor-converted white light-emitting diodes with high color rendering index. Opt Express 23:A1024–A1029CrossRefGoogle Scholar
Chen KJ, Lai YC, Lin BC et al (2015) Efficient hybrid white light-emitting diodes by organic-inorganic materials at different CCT from 3000 K to 9000 K. Opt Express 23:A204–A210CrossRefGoogle Scholar
Gao Z, Sun C, Liu H et al (2019) White light-emitting diodes based on carbon dots and Mn-doped CsPbxMn1-xCl3 nanocrystals. Nanotechnology 30:245201–245205CrossRefGoogle Scholar
Lan C, Zhou Z, Wei R et al (2019) Two-dimensional perovskite materials: from synthesis to energy-related applications. Materials today energy 11:61–82CrossRefGoogle Scholar
Al-Amri AM, Cheng B, He J-H et al (2019) Perovskite methylammonium lead trihalide heterostructures: progress and challenges. IEEE Trans Nano 18:1–12CrossRefGoogle Scholar
Zhao D, Wang C, Song Z et al (2018) Four-terminal all-perovskite tandem solar cells achieving power conversion efficiencies exceeding 23%. ACS Energy Lett 3:305–306CrossRefGoogle Scholar
Zhang Y, Xu W, Xu X et al (2019) Self-powered dual-color UV-green photodetectors based on SnO2 millimeter wire and microwires/CsPbBr3 particle heterojunctions. J Phys Chem Lett 10:836–841CrossRefGoogle Scholar
Lin CH, Cheng B, Li TY et al (2019) Orthogonal lithography for halide perovskite optoelectronic nanodevices. ACS Nano 13:1168–1176Google Scholar
Dong R, Lan C, Xu X et al (2018) A novel series of quasi-2D Ruddlesden-Popper perovskites based on short-chained spacer cation for enhanced photodetection. ACS Appl Mater Inter 10:19019–19026CrossRefGoogle Scholar
Yakunin S, Protesescu L, Krie F et al (2015) Low-threshold amplified spontaneous emission and lasing from colloidal nanocrystals of caesium lead halide perovskites. Nat Commun 6:8056–8062CrossRefGoogle Scholar
Protesescu L, Yakunin S, Bodnarchuk MI et al (2015) Nanocrystals of cesium lead halide perovskites (CsPbX3, X = Cl, Br, and I): novel optoelectronic materials showing bright emission with wide color gamut. Nano Lett 15:3692–3696CrossRefGoogle Scholar
Ramasamy P, Lim DH, Kim B et al (2016) All-inorganic cesium lead halide perovskite nanocrystals for photodetector applications. Chem Commun 52:2067–2070CrossRefGoogle Scholar
Bai S, Yuan Z, Gao F et al (2016) Colloidal metal halide perovskite nanocrystals: synthesis, characterization, and applications. Mater Chem 4:3898–3904Google Scholar
Sun C, Gao Z, Liu H et al (2018) A new method to discover the reaction mechanism of perovskite nanocrystals. Dalton Trans 47:16218–16224CrossRefGoogle Scholar
Sun C, Su S, Gao Z et al (2019) Stimuli-responsive inks based on perovskite quantum dots for advanced full-color information encryption and decryption. ACS Appl Mater Inter 11:8210–8216CrossRefGoogle Scholar
Sun C, Zhang Y, Ruan C et al (2016) Efficient and stable white LEDs with silica-coated inorganic perovskite quantum dots. Adv Mater 28:10088–10094CrossRefGoogle Scholar
Shen X, Sun C, Bai X et al (2018) Efficient and stable CsPb (Br/I)3@anthracene composites for white light-emitting devices. ACS Appl Mater Inter 10:16768–16775CrossRefGoogle Scholar
Zhou Q, Bai Z, Lu WG et al (2016) In situ fabrication of halide perovskite nanocrystal-embedded polymer composite films with enhanced photoluminescence for display backlights. Adv Mater 28:9163–9168CrossRefGoogle Scholar
Chen YM, Zhou Y, Zhao Q et al (2018) Cs4PbBr6/CsPbBr3 Perovskite composites with near-unity luminescence quantum yield: large-scale synthesis, luminescence and formation mechanism, and white light-emitting diode application. ACS Appl Mater Inter 10:15905–15912CrossRefGoogle Scholar
Li X, Wu Y, Zhang S et al (2016) CsPbX3 quantum dots for lighting and displays: room-temperature synthesis, photoluminescence superiorities, underlying origins and white light-emitting diodes. Adv Funct Mater 26:2435–2445CrossRefGoogle Scholar
Li Y, Lv Y, Guo Z et al (2018) One-step preparation of long-term stable and flexible CsPbBr3 perovskite quantum dots/ethylene vinyl acetate copolymer composite films for white light-emitting diodes. ACS Appl Mater Inter 10:15888–15894CrossRefGoogle Scholar
Dohner ER, Jaffe A, Bradshaw LR et al (2014) Intrinsic white-light emission from layered hybrid perovskites. J Am Chem Soc 136:13154–13157CrossRefGoogle Scholar
Yuan Z, Zhou C, Messier J et al (2016) A microscale perovskite as single component broadband phosphor for downconversion white-light-emitting devices. Adv Opt Mater 4:2009–2015CrossRefGoogle Scholar
Thirumal K, Chong WK, Xie W et al (2017) Morphology-independent stable white-light emission from self-assembled two-dimensional perovskites driven by strong exciton–phonon coupling to the organic framework. Chem Mater 29:3947–3953CrossRefGoogle Scholar
Wang A, Guo Y, Muhammad F et al (2017) Controlled synthesis of lead-free cesium tin halide perovskite cubic nanocages with high stability. Chem Mater 29:6493–6501CrossRefGoogle Scholar
Zhu X (2016) The perovskite fever and beyond. Acc Chem Res 49:355–356CrossRefGoogle Scholar
Swarnkar A, Ravi VK, Nag A et al (2017) Beyond colloidal cesium lead halide perovskite nanocrystals: analogous metal halides and doping. ACS Energy Lett 2:1089–1098CrossRefGoogle Scholar
Stoumpos CC, Frazer L, Clark DJ et al (2015) Hybrid germanium iodide perovskite semiconductors: active lone pairs, structural distortions, direct and indirect energy gaps and strong nonlinear optical properties. J Am Chem Soc 137:6804–6819CrossRefGoogle Scholar
McClure ET, Ball MR, Windl W et al (2016) Cs2AgBiX6(X = Br, Cl): new visible light absorbing, lead-free halide perovskite semiconductors. Chem Mater 28:1348–1354CrossRefGoogle Scholar
Liu H, Wu Z, Shao J et al (2017) CsPbxMn1-xCl3 perovskite quantum dots with high Mn substitution ratio. ACS Nano 11:2239–2247CrossRefGoogle Scholar
Parobek D, Roman BJ, Dong Y et al (2016) Exciton-to-dopant energy transfer in Mn-doped cesium lead halide perovskite nanocrystals. Nano Lett 16:7376–7380CrossRefGoogle Scholar
Tan Z, Li J, Zhang C et al (2018) Highly efficient blue-emitting Bi-doped Cs2SnCl6 perovskite variant: photoluminescence induced by impurity doping. Adv Funct Mater 28:1801131–1801140CrossRefGoogle Scholar
Liu W, Lin Q, Li H et al (2016) Mn2+-doped lead halide perovskite nanocrystals with dual-color emission controlled by halide content. J Am Chem Soc 138:14954–14961CrossRefGoogle Scholar
Das AS, Dutta SK, Dutta A et al (2017) Chemically tailoring the dopant emission in manganese-doped CsPbCl3 perovskite nanocrystals. Angew Chem Int Ed 56:8746–8750CrossRefGoogle Scholar
Chen D, Fang G, Chen X et al (2017) Silica-coated Mn-doped CsPb (Cl/Br)3 inorganic perovskite quantum dots: exciton-to-Mn energy transfer and blue-excitable solid-state lighting. ACS Appl Mater Inter 9:40477–40487CrossRefGoogle Scholar
Tian Z, Zhang X, Li D et al (2017) Full-color inorganic carbon dot phosphors for white-light-emitting diodes. Adv Opt Mater 5:1700416–1700424CrossRefGoogle Scholar
Zhu J, Bai X, Bai J et al (2018) Emitting color tunable carbon dots by adjusting solvent towards light-emitting devices. Nanotechnology 29:085705–085712CrossRefGoogle Scholar
Sun C, Zhang Y, Kalytchuk S et al (2015) Down-conversion monochromatic light-emitting diodes with the color determined by the active layer thickness and concentration of carbon dots. J Mater Chem C 3:6613–6615CrossRefGoogle Scholar
Shao H, Bai X, Pan G et al (2018) Highly efficient and stable blue-emitting CsPbBr3@SiO2 nanospheres through low temperature synthesis for nanoprinting and WLED. Nanotechnology 29:285706–285714CrossRefGoogle Scholar
Pan G, Bai X, Xu W et al (2018) Impurity ions codoped cesium lead halide perovskite nanocrystals with bright white light emission toward ultraviolet-white light-emitting diode. ACS Appl Mater Inter 10:39040–39048CrossRefGoogle Scholar
Zhang M, Wang M, Yang Z et al (2018) Preparation of all-inorganic perovskite quantum dots-polymer composite for white LEDs application. J Alloy Compd 748:537–545CrossRefGoogle Scholar
Zhang F, Shi ZF, Ma ZZ et al (2018) Silica coating enhances the stability of inorganic perovskite nanocrystals for efficient and stable down-conversion in white light-emitting devices. Nanoscale 10:20131–20139CrossRefGoogle Scholar
Liu S, Shao G, Ding L et al (2019) Sn-doped CsPbBr3 QDs glasses with excellent stability and optical properties for WLED. Chem Eng J 361:937–944CrossRefGoogle Scholar
Zhao B, Bai S, Kim V et al (2018) High-efficiency perovskite–polymer bulk heterostructure light-emitting diodes. Nat Photonics 12:783–789CrossRefGoogle Scholar
Tang SY, Medina H, Yen YT et al (2019) Enhanced photocarrier generation with selectable wavelengths by M-decorated-CuInS2 nanocrystals (M = Au and Pt) synthesized in a single surfactant process on MoS2 bilayers. Small 15:1803529–1803537CrossRefGoogle Scholar
Ye S, Y M, Yan W et al (2017) Enhanced photoluminescence of CsPbBr3@Ag hybrid perovskite quantum dots. J Mater Chem C 5:8187–8193CrossRefGoogle Scholar
Zhang X, Lu M, Zhang Y et al (2018) PbS capped CsPbI3 nanocrystals for efficient and stable light-emitting devices using p-i-n structures. ACS Central Sci 4:1352–1359CrossRefGoogle Scholar
Shi Z, Li Y, Li S et al (2018) Localized surface plasmon enhanced all-inorganic perovskite quantum dot light-emitting diodes based on coaxial core/shell heterojunction architecture. Adv Funct Mater 28:1707031–1707041CrossRefGoogle Scholar
© The Author(s). 2019
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
Authors and Affiliations
Hanxin Liu1Chun Sun1Email authorView author's OrcID profileZhiyuan Gao1Chong Geng1Shuangshuang Shi1Le Wang1Sijing Su1Wengang Bi1Email author1.Tianjin Key Laboratory of Electronic Materials and Devices, School of Electronics and Information EngineeringHebei University of TechnologyTianjinPeople’s Republic of China